Internal CO2 Corrosion of Mild Steel Pipelines under Inert Solid Deposits
Jin Huang, Bruce Brown, Xiu Jiang, Brian Kinsella and Srdjan Nesic1
Institute for Corrosion and Multiphase Technology, Ohio University
342 west state street, Athens, OH, 45701
Under-deposit CO2 corrosion occurs when solids like sand, corrosion products, wax or a variety
of other particles deposit on the bottom of pipelines, forming a bed or layer of solids1,2. Under-
deposit CO2 corrosion is different from “regular” CO2 corrosion as the aqueous solution beneath
the solids is chemically and physically different from the “bulk” solution in the pipe. The
presence of solids can also limit inhibitor access to the metal surface which can initiate severe
localized corrosion 3.
Initial testing was directed towards defining and modeling the fundamental mild steel CO2
corrosion mechanisms occurring in the presence of clean inert solid deposits with different
particle sizes and shapes (SiO2 powder, glass beads (GB) and sand). Experiments were
conducted in a glass cell at a total pressure of 1 bar for temperatures of 25°C and 80°C. The mild
steel sample was immersed in 1 wt% NaCl electrolyte for one day. Corrosion behavior was
characterized by electrochemical techniques, including LPR (linear polarization resistance), EIS
(electrochemical impedance spectroscopy) and potentiodynamic sweeps. Steel surface
morphologies have been analyzed by using SEM (scanning electron microscope) and EDX
(energy dispersive x-ray).
Keywords: solids, under-deposit, CO2 corrosion, mild steel, pipelines
1 Corresponding author email address: email@example.com (S. Nesic)
©2010 by NACE International. Requests for permission to publish this manuscript in any form, in part or in whole, must be in writing to NACE
International, Publications Division, 1440 South Creek Drive, Houston, Texas 77084. The material presented and the views expressed in this paper are
solely those of the author(s) and are not necessarily endorsed by the Association.
Severe corrosion problems such as crevice corrosion and pitting can be found under solid
deposits in pipelines 2. Localized corrosion occurs under these deposits because they provide a
region that is chemically and physically different from the rest of the steel surface which is not
covered 4. This difference may generate a galvanic corrosion cell or affect inhibitor performance
or provide ideal conditions for bacterial growth 3. Under-deposit corrosion is prevalent at the
bottom of horizontal lines where flow rates are not large enough to keep the solids suspended.
However, no work is reported in the open literature that covers the mechanisms of under-deposit
corrosion as most of literature refers to the effect of deposits on inhibitor performance4,5,6.
Pedersen, et al.5 developed a test method for studying under-deposit corrosion and investigated
the inhibitor performance under sand deposits. Their work, while being useful in many ways,
does not focus on the mechanism of the corrosion process under the deposit.
The goal of this work is to gain an initial understanding of the CO2 corrosion mechanism of mild
steel covered by inert deposits by experimentally studying the effects of deposit porosity, deposit
thickness, solution pH, and temperature and by deploying the in-situ electrochemical and
techniques. The effect of the deposits on inhibitor performances and potential galvanic effects
related to under-deposit corrosion were not covered in this stage of the project.
All tests were conducted in a glass cell using a standard three-electrode set up, as shown in
Figure 1. The glass cell was filled with 2 liters of DI water with 1%wt NaCl . X65 mild steel was
used as the working electrode (WE) for electrochemical measurements. Platinum wire was used
as a counter electrode (CE) and a saturated silver-silver chloride (Ag/AgCl) electrode was used
as a reference electrode (RE).
Electrochemical techniques including linear polarization resistance (LPR), potentiodynamic
sweeps (PDS) and electrochemical impedance spectroscopy (EIS) were used to measure the
corrosion rate and identify the corrosion mechanisms of mild steel both with and without solid
deposits. The WE was polarized ±5mV from open circuit potential (Eoc) during the LPR
measurements at a scan rate of 0.125mV/s to obtain the polarization resistance Rp, which was
then used to calculate the general corrosion rate of mild steel. For the EIS measurement, a
sinusoidal potential signal ±5mV peak-to-peak around Eoc was applied to the WE, scanning from
10kHz to 1mHz. This scan enables the identification of both the solution resistance (Rs) – at the
highest frequency range and the “fingerprint” of the various reactions involved in the corrosion
process – at the lower frequency ranges. Corrosion mechanisms were also studied by using
potentiodynamic sweeps which were conducted in two steps. Polarization of the WE started
from Eoc by sweeping the potential at a scan rate of 0.125mV/s in the cathodic (more negative)
direction by 0.4V, and then disconnecting and pausing until stable Eoc was attained again, when
the potential of the WE was swept in the anodic (more positive) direction by 0.2V using the same
Conditions for the under-deposit corrosion experiments are summarized in the test matrix
outlined in Table 1. Before being immersed into the electrolyte, the WE surface was polished by
using 200, 400 and 600 grit silica carbide (SiC) paper wetted with water, then rinsed with
isopropanol, and air dried. The electrolyte in the glass cell was purged continuously with CO2
during each test to maintain the CO2 partial pressure and remove dissolved oxygen. Separate
measurements have proven that this experimental setup/procedure ensures that the concentration
of dissolved oxygen does not exceed 20 ppb what is considered acceptable.
Baseline experiments included corrosion measurements on “bare” mild steel and under-deposit
corrosion tests as outlined the test matrix shown in Table 1. Before each under-deposit
experiment, the steel sample was immersed in the electrolyte for about one hour without a
deposit, where the bare corrosion rate and solution resistance were measured by LPR and EIS, to
ensure that similar initial surface conditions were achieved before each experiment. Then the
deposit was introduced and test was carried out for a further 24 hours.
Corroded steel surface morphologies and composition have been analyzed by using SEM and
EDX. Surface pH measurements were also conducted by using a specially designed surface pH
probe7, which confirmed that a different pH is found under the solid deposit layer.
Testing sample holder
All corrosion samples were cylindrical, made from X65 mild steel, with a surface area of 8 cm2
(0.0008 m2) and height of 6.35 mm. The samples were mounted in a specially designed sample
holder, where only the top surface of the steel sample was exposed to the environment with an
O-ring separating the rest of the cylinder from the corrosive environment. At the bottom surface
of the steel sample, spring loaded gold contact pins are used for electrochemical connections.
The cylindrical steel sample and the sample holder are shown in Figure 2.
The deposit types used in this work were sand, powder and glass beads. All of these deposits are
the same base material, i.e. silica dioxide SiO2. The main difference between them is their grain
size and shape, as can be seen in SEM images shown in Figure 3. The deposit porosity was
experimentally determined. For each deposit, a specific amount of DI water Vwater (ml) was
added to dry deposit Vs (ml), the total volume of deposit and DI water Vtotal was recorded and
porosity then was calculated:
The different grain sizes result in different physical properties, which are listed in Table 2.
All deposits used in this work were cleaned by 1 M sodium hydroxide solution, 5 M HCl acid
solution and DI water to remove possible impurities before being used. The deposit was
submerged in a 1wt% NaCl solution and stored in a separate beaker purged by CO2 to remove
dissolved oxygen. The pH of the deposit-electrolyte solution was also adjusted by NaHCO3
solution to the same pH as the testing electrolyte. After the test sample was pre-corroded for
about one hour, the cleaned deposit was transferred by a Pipet to the glass cell.
RESULTS AND DISCUSSION
Effect of deposit porosity and deposit thickness
It is seen in Figure 4 that introducing a deposit on the steel surface caused a sudden decrease in
the corrosion rate by a factor 2 to 4 and then remained stable for 24 hours. The first data point of
each data set was recorded before the deposit was introduced which shows repeatability of the
initial condition. The corrosion rate data indicates that the more porous the deposit, the more the
steel corroded as would be expected. As a first approximation, a linear relationship between
corrosion rate and deposit porosity was found, see Figure 5. The corresponding corrosion
potential change was also recorded, as seen in Figure 6. As compared to a bare steel, the
corrosion potential increased by about 10-20mV for different deposits. The potentiodynamic
sweeps measurements done at the end of the test after 24 hours are, shown in Figure 7. It can be
seen that both ano